A second-order nonlinear optical material with a 5-fold interpenetrating diamondoid framework based on two achiral precursors: spontaneous resolution to absolute chiral induction.
Shi, Zhenzhen; Qin, Ling; Zheng, Hegen; Dalton transactions (Cambridge, England : 2003) 46 (2017) 4589–4594; doi:10.1039/c7dt00614d

data_7042429
_publ_section_title
;
 A second-order nonlinear optical material with a 5-fold interpenetrating
 diamondoid framework based on two achiral precursors: spontaneous
 resolution to absolute chiral induction.
;
_journal_issue                   14
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              4589
_journal_page_last               4594
_journal_paper_doi               10.1039/c7dt00614d
_journal_volume                  46
_journal_year                    2017
_chemical_formula_moiety         'C96 H78 N22 O10 Zn2'
_chemical_formula_sum            'C96 H78 N22 O10 Zn2'
_chemical_formula_weight         1830.54
_space_group_crystal_system      orthorhombic
_space_group_IT_number           19
_space_group_name_Hall           'P 2ac 2ab'
_space_group_name_H-M_alt        'P 21 21 21'
_symmetry_space_group_name_Hall  'P 2ac 2ab'
_symmetry_space_group_name_H-M   'P 21 21 21'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2016/4
_audit_update_record
;
2016-11-30 deposited with the CCDC.
2017-03-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.3272(10)
_cell_length_b                   21.377(2)
_cell_length_c                   21.377
_cell_measurement_reflns_used    9928
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.206
_cell_measurement_theta_min      2.382
_cell_volume                     4262.3(6)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2016/4 (Sheldrick, 2016)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0550
_diffrn_reflns_av_unetI/netI     0.0554
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            34936
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.361
_diffrn_reflns_theta_min         2.130
_exptl_absorpt_coefficient_mu    0.639
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.426
_exptl_crystal_description       rod
_exptl_crystal_F_000             1896
_exptl_crystal_size_max          0.280
_exptl_crystal_size_mid          0.080
_exptl_crystal_size_min          0.070
_exptl_transmission_factor_max   0.956
_exptl_transmission_factor_min   0.940
_refine_diff_density_max         0.620
_refine_diff_density_min         -0.426
_refine_diff_density_rms         0.062
_refine_ls_abs_structure_details
; 
 Refined as an inversion twin. 
;
_refine_ls_abs_structure_Flack   0.013(13)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.035
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     590
_refine_ls_number_reflns         8720
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.035
_refine_ls_R_factor_all          0.0496
_refine_ls_R_factor_gt           0.0414
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0468P)^2^+1.4882P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0949
_refine_ls_wR_factor_ref         0.0985
_reflns_Friedel_coverage         0.792
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                7663
_reflns_number_total             8720
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7dt00614d2.cif
_cod_data_source_block           2
_cod_depositor_comments
'Adding full bibliography for 7042428--7042429.cif.'
_cod_original_cell_volume        4262.5(6)
_cod_database_code               7042429
_shelx_shelxl_version_number     2016/4
_shelx_estimated_absorpt_t_min   0.841
_shelx_estimated_absorpt_t_max   0.957
_shelx_res_checksum              7470